#------------------------------------------------------------------------------
#$Date: 2024-04-25 17:59:02 +0300 (Thu, 25 Apr 2024) $
#$Revision: 291351 $
#$URL: file:///home/coder/svn-repositories/cod/cif/9/00/43/9004304.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the American Mineralogist Crystal Structure Database,
# http://rruff.geo.arizona.edu/AMS/amcsd.php
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_9004304
loop_
_publ_author_name
'Caucia, F.'
'Callegari, A.'
'Oberti, R.'
'Ungaretti, L.'
'Hawthorne, F. C.'
_publ_section_title
;
 Structural aspects of oxidation-dehydrogenation in staurolite
 Sample: T = 900 C
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              477
_journal_page_last               489
_journal_volume                  32
_journal_year                    1994
_chemical_formula_sum            'Al4.8 Fe0.83 H Mg0.19 O12 Si1.9 Zn0.01'
_chemical_name_mineral           Staurolite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.00
_cell_angle_gamma                90
_cell_length_a                   7.860
_cell_length_b                   16.645
_cell_length_c                   5.606
_cell_formula_units_Z            4
_cell_volume                     733.431
_database_code_amcsd             0005377
_diffrn_ambient_temperature      1173.15
_exptl_crystal_density_diffrn    3.872
_cod_original_formula_sum        'Si1.9 Al4.8 Fe.83 Zn.01 Mg.19 O12 H'
_cod_database_code               9004304
loop_
_space_group_symop_operation_xyz
x,y,z
1/2+x,1/2+y,z
x,-y,z
1/2+x,1/2-y,z
-x,y,-z
1/2-x,1/2+y,-z
-x,-y,-z
1/2-x,1/2-y,-z
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_U_iso_or_equiv
SiT1 0.13490 0.16817 0.24998 0.95000 0.00532
AlT1 0.13490 0.16817 0.24998 0.05000 0.00532
FeT2 0.38022 0.00000 0.25007 0.40000 0.00747
ZnT2 0.38022 0.00000 0.25007 0.01000 0.00747
MgT2 0.38022 0.00000 0.25007 0.08000 0.00747
AlT2 0.38022 0.00000 0.25007 0.18000 0.00747
FeT3 0.12589 0.00000 0.25012 0.09000 0.00633
AlT3 0.12589 0.00000 0.25012 0.20000 0.00633
AlM1A 0.50000 0.17339 0.00000 0.97000 0.00532
FeM1A 0.50000 0.17339 0.00000 0.03000 0.00532
AlM1B 0.50000 0.17338 0.50000 0.97000 0.00532
FeM1B 0.50000 0.17338 0.50000 0.03000 0.00532
AlM2 0.26421 0.41261 0.24999 0.92000 0.00722
FeM2 0.26421 0.41261 0.24999 0.08000 0.00722
AlM3A 0.00000 0.00000 0.00000 0.54000 0.00608
MgM3A 0.00000 0.00000 0.00000 0.04000 0.00608
FeM3A 0.00000 0.00000 0.00000 0.06000 0.00608
AlM3B 0.00000 0.00000 0.50000 0.54000 0.00608
MgM3B 0.00000 0.00000 0.50000 0.04000 0.00608
FeM3B 0.00000 0.00000 0.50000 0.06000 0.00608
FeM4A 0.50000 0.00000 0.00000 0.06000 0.01115
MgM4A 0.50000 0.00000 0.00000 0.07000 0.01115
FeM4B 0.50000 0.00000 0.50000 0.06000 0.01153
MgM4B 0.50000 0.00000 0.50000 0.07000 0.01153
O1A 0.23849 0.00000 0.97081 0.50000 0.01127
O-H1A 0.23849 0.00000 0.97081 0.50000 0.01127
O1B 0.23862 0.00000 0.52906 0.50000 0.01102
O-H1B 0.23862 0.00000 0.52906 0.50000 0.01102
O2A 0.25573 0.16200 0.01427 1.00000 0.00608
O2B 0.25572 0.16198 0.48573 1.00000 0.00608
O3 0.00353 0.09094 0.24983 1.00000 0.00899
O4 0.02112 0.25059 0.25013 1.00000 0.00583
O5 0.52428 0.09755 0.25002 1.00000 0.00659
loop_
_cod_related_entry_id
_cod_related_entry_database
_cod_related_entry_code
1 AMCSD 0005377
